OPEN ACCESS

materials ISSN 1996-1944 www.mdpi.com/journal/materials Article

Effect of Stress Amplitude on the Damping of Recycled Aggregate Concrete Chaofeng Liang 1 , Tiejun Liu 2, *, Jianzhuang Xiao 3 , Dujian Zou 2 and Qiuwei Yang 1 1

Department of Civil Engineering, Shaoxing University, Shaoxing 312000, China; E-Mails: [email protected] (C.L.); [email protected] (Q.Y.) 2 Shenzhen Graduate School, Harbin Institute of Technology, Shenzhen 518055, China; E-Mail: [email protected] 3 Department of Structural Engineering, Tongji University, Shanghai 200092, China; E-Mail: [email protected] * Author to whom correspondence should be addressed; E-Mail: [email protected]; Tel.: +86-755-2603-3368; Fax: +86-755-2603-3509. Academic Editor: Jorge de Brito Received: 23 July 2015 / Accepted: 11 August 2015 / Published: 14 August 2015

Abstract: Damping characterizes the energy dissipation capacity of materials and structures, and it is affected by several external factors such as vibrating frequency, stress history, temperature, and stress amplitude. This study investigates the relationship between the damping and the stress amplitude of environment-friendly recycled aggregate concrete (RAC). First, a function model of a member’s loss factor and stress amplitude was derived based on Lazan’s damping-stress function. Then, the influence of stress amplitude on the loss tangent of RAC was experimentally investigated. Finally, parameters used to determine the newly derived function were obtained by numerical fitting. It is shown that the member’s loss factor is affected not only by the stress amplitude but also by factors such as the cross section shapes, boundary conditions, load types, and loading positions. The loss tangent of RAC increases with the stress amplitude, even at low stress amplitude. The damping energy exponent of RAC is not identically equal to 2.0, indicating that the damping is nonlinear. It is also found that the energy dissipation capacity of RAC is superior to that of natural aggregate concrete (NAC), and the energy dissipation capacity can be further improved by adding modified admixtures.

Materials 2015, 8

5299

Keywords: stress amplitude-dependent damping; loss factor; recycled aggregate concrete; damping energy coefficient; damping energy exponent

1. Introduction Damping reflects energy dissipation, and it is one of the intrinsic dynamic characteristics of a material. It strongly affects a structure’s dynamic response and damage evolution. Thus far, a uniform understanding of damping that explains its complex mechanism in detail has not been obtained. Concrete is a brittle material consisting of a three-phase medium: coarse aggregate, cement matrix, and interfacial transition zone (ITZ). Every component has a significant effect on the damping of concrete. Many studies have focused on the influence of admixtures on the damping of concrete; however, few studies have investigated the influence of coarse aggregate, especially recycled coarse aggregate (RCA). Chung et al. [1–4] studied the damping capacity and storage modulus of cement paste and mortar with silica fume, latex, methycellulose, and graphite as admixtures. Neithalath et al. [5] investigated the influence of morphologically altered cellulose fibers on the acoustic and damping characteristics of cement mortar. It should be noted that most studies focused on enhanced damping by admixtures at the material level. In contrast, Ou et al. [6,7] conducted experimental studies at the structural level. The dynamic response of reinforced concrete (RC) structures with vibration-reducing admixtures was studied by shaking table and uniaxial hysteretic experiments. Swamy and Rigby [8] and Jordan [9] found that the influence of the addition of aggregate inclusions on the damping capacity of the mortar matrix depended on the volume content of the aggregate, the degree of hydration, and the state of curing, and that the addition of coarse aggregate reduced the damping of mortar. Ke et al. [10] experimentally investigated the damping ratio of concrete cantilever and found that the damping ratio increased remarkably after the surface of natural coarse aggregates was covered with viscoelastic materials (e.g., asphalt), and concluded that the weaker interface between the treated surface of natural coarse aggregate and cement mortar increased the interfacial viscous sliding during vibration. External conditions such as vibration frequency, stress history, temperature, and stress amplitude influence damping. Among these, stress amplitude is one of the important factors influencing damping, especially for concrete materials. Lazan [11] found that many building materials were not completely elastic even when their stress was low, and their stress-strain curves formed hysteresis loops. Through numerous experimental investigations, he provided a damping-stress function (Equation (A1)) that described the power relationship between the damping energy and the stress. Moreover, the damping energy coefficient and the exponent of the damping-stress function have been determined for some materials such as mild steel but not for concrete. Kume et al. [12] evaluated the loss factor of a cantilever steel beam in terms of Lazan’s damping-stress function. In their study, the stress distribution function was determined by the quasi-static deformation in the cantilever beam as given by the solution for undamped forced vibration. However, the stress distribution function can only be derived theoretically for simple structural members. Therefore, Gounaris et al. [13,14] combined the finite element method and the numerical iterative technique with Lazan’s damping-stress function to calculate the nonlinear material damping of complex members. Furthermore, the parameters of the damping-stress function for mild steel were determined by a newly developed method called the iterative complex eigensolution method.

Materials 2015, 8

5300

Jordan [9] investigated the effect of stress, frequency, mix, and age on the damping of concrete and found that wet concrete showed a steady increase in damping with an increase in the maximum stress. Hwang et al. [15] experimentally determined the effect of the displacement history sequence and magnitude on the cyclic response of reinforced flexural members and found that the energy dissipation capacity was a function of the applied stress intensity and the magnitude of maximum displacements applied to the members. Darwin et al. [16] studied the energy dissipation index of RC beams with different geometries under cyclic load and found that it was primarily controlled by the maximum stress, concrete strength, and transverse steel capacity. Wang et al. [17] presented a new method to calculate the material damping of RC components in the elastic stage under axial cyclic load; furthermore, they established a relation formula for the energy dissipation of RC beams with maximum stress amplitude, concrete strength, and reinforcement ratio through nonlinear regression. Jeary et al. [18,19] employed a time series analysis method to obtain the relationship between structural damping and vibration amplitude at high amplitude level, and took the fracture at both microscopic and macroscopic scale into consideration. Li et al. [20,21] emphasized that the effect of amplitude-dependent damping on the dynamic responses of a super tall building was significant and that the knowledge of the actual damping characteristics was very important for the accurate prediction of wind-induced vibrations in such buildings. The recycled aggregate concrete incorporates recycled aggregates produced from construction and demolition wastes, and it is an environment-friendly building material. Therefore, the use of recycled aggregates as structural grade concrete has generated extensive interest in civil engineering construction. However, the recycled aggregate always has a lot of mortar on the surface and internal micro-cracks [22,23]. The shape and amount of micro-cracks existing in recycled aggregate deteriorate the mechanical properties of RAC, such as compressive and tensile strength [24–27]. Due to the intrinsic porosity of RA, the durability of RAC is worse than that of NAC [28,29]. The creep and drying shrinkage of RAC increase significantly due to the lower elastic modulus of RA [30,31]. The fatigue life of RAC is lower than that of NAC for the same stress level under cyclic bend loading and the dynamic compressive strength decreases with an increasing RA replacement ratio at high strain rates [32,33]. The nature and initial moisture condition of RA determine the microstructural characteristics of the aggregate–cement paste interface and the mechanical properties of the ITZ [34,35]. Currently, a large number of studies have been carried out to evaluate the mechanical properties, durability, and volume stability of RAC. Nonetheless, the studies on the damping property of RAC are still very few. So far, most reported experimental investigations and numerical analyses concerning stress amplitude-dependent damping show that high stress amplitude has a very significant influence on damping. However, few studies have focused on the stress amplitude-dependent damping function of widely used concrete materials at low stress amplitudes, especially for recycled aggregate concrete. As a refined constitutive model is increasingly important for the safety and serviceability assessment of RC structures during vibration induced by wind or earthquake, damping at low stress amplitudes should be discussed in detail. In this study, an expression for the loss factor and bending stress amplitude was established based on Lazan’s damping-stress function, and an experimental investigation was conducted to study the loss tangent of RAC at a low stress amplitude. In addition, the damping energy coefficient

Materials 2015, 8

5301

Materials 2015, 8 to determine the stress amplitude-dependent damping function of RAC were obtained 5290 and exponent used by numerical fitting. and exponent used to determine the stress amplitude-dependent damping function of RAC were obtained 2. Theoretical Derivation by numerical fitting. 2.1. Material Damping Models 2. Theoretical Derivation damping-stress function is given as 2.1.Lazan’s Material Damping Models n Lazan’s damping-stress function is given asDe “ Jσa

(1)

De Jσ na where De is the damping energy per cycle for a unit volume of material; σa is the stress; J and n are(1) the damping coefficientenergy and exponent, Deenergy where is the damping per cyclerespectively. for a unit volume of material; σ a is the stress; J and n are and Garrick’s damping model [36] is convenient for describing viscoelastic theTheodorsen damping energy coefficientcomplex and exponent, respectively. material behavior, its damping parameters canmodel be easily experimentally. This damping Theodorsen andand Garrick’s complex damping [36]determined is convenient for describing viscoelastic model is behavior, therefore widely and parameters it is given ascan be easily determined experimentally. This damping material and its used, damping

model is therefore widely used, and it is˚ given as 2 σ “ E ε “ pE ` iE qε “ p1 ` iηqEε (2) * E ( E iE ) (1 i) E (2) 2 where E ˚*, E, and E are the complex modulus, elastic modulus, and loss modulus, respectively; η is the where E , E , and E are the complex modulus, elastic modulus, and loss modulus, respectively; loss tangent; σ, ε are the bending stress and strain, respectively. is the loss tangent; σ , are the bending stress and strain, respectively. 2.2. Member Model and Assumptions 2.2. Member Model and Assumptions Figure 1 shows the member model with a constant cross section, and its boundary conditions are Figure 1 shows the member model with a constant cross section, and its boundary conditions are arbitrary. The following assumptions are made: arbitrary. The following assumptions are made: (1) The load load types types (1) The The member member isis only only loaded loaded in in the the YY direction direction and and bent bent inin the the XOY XOY plane. plane. The are arearbitrary. arbitrary. (2) The about thethe Y-axis, and and the bending stressstress is uniform along the Z-axis (2) Thecross crosssection sectionis issymmetric symmetric about Y-axis, the bending is uniform along the of the cross section. The cross section shape is arbitrary. Z-axis of the cross section. The cross section shape is arbitrary. (3) The influence of shear (3) Thetransverse transversebending bending vibration vibration is is the the member’s member’s main main vibration vibration mode, mode, and and the the influence of shear stress stresson ondamping dampingisisneglected. neglected. (4) (4) The Thematerial materialisisconsidered consideredcontinuous continuousand andisotropic, isotropic,and andthe thebending bendingstress stressamplitude amplitudeisislow. low.

Figure 1. Member model with constant cross section. Figure 1. Member model with constant cross section.

Materials 2015, 8

5302

2.3. Elastic Strain Energy of Member The elastic strain energy for a unit volume of the member Ue , as shown in Figure 1, is defined as pσax qy 2 Ue “ 2E

(3)

where pσax qy is the bending stress at coordinates (x, y); y, the distance from the neutral axis of the member’s cross section; and x, the coordinate along the longitudinal axis of the member. The elastic strain energy of the global member Us is obtained as ¨ h ˛¨ l ˛ ˙2 ˆ 2 ˙ ż1 ż ˆ ż ĳ σax 1 σam 2 ‚˝ 1 plAq ˝ y 2 zh´ dx‚ Us “ Ue dV “ Ue zdxdy “ (4) i dy 2E A l σam V

Ω

0

´ h2

l

where A is the member’s cross-sectional area; l is the effective length of the member; h1 and h2 are the distance from the top and bottom edge to the neutral axis, respectively; hi is the greater of h1 and h2 ; z is the width of the cross section at coordinates (x, y); σax “ pσax qy ˆ hi {y

(5)

is the maximum bending stress amplitude of the cross section at coordinate x; and σam is the maximum bending stress of the whole member. Moreover, we define Uam

σ2 “ am , 2E

Vs “ lA ,

1 χc “ A

żh1

1 2 y 2 zh´ i dy, „and χl “ l

żl ˆ

σax σam

˙2 dx

(6)

0

´ h2

where Uam is the maximum elastic strain energy; Vs is the entire volume; χc and χl are the cross section factor and length factor for the member’s elastic strain energy, respectively. Then, the elastic strain energy of the global member can be simply written as Us “ Uam Vs χc χl

(7)

2.4. Damping Energy of Member According to Equation (1), the damping energy of a unit volume at coordinates (x, y) can be expressed as De “ Jpσax qny (8) The damping energy of the global member Ds is obtained as ˛¨ l ˛ ¨ h ˙n ż1 ż ˆ ż ĳ 1 1 σax n Ds “ De dV “ De zdxdy “ pJσnam q pAlq ˝ y n zh´ dy ‚˝ dx‚ i A l σam V

Ω

´ h2

0

(9)

Materials 2015, 8

5303

We define Dam

1 “ Jσnam , γc “ A

żh1

1 n dy, and γl “ y n zh´ i l

żl ˆ

σax σam

˙n dx

(10)

0

´ h2

where Dam is the maximum damping energy for unit volume of the member, and γc and γl are the cross section factor and length factor for the member’s damping energy, respectively. Then, the damping energy of the global member takes the form Ds “ Dam Vs γc γl

(11)

2.5. Loss Factor of Member The member’s loss factor ηs is defined as ηs “

Ds 2πUs

(12)

By substituting Equations (6) and (10) into Equation (11) and taking into account Equations (5) and (9), the member’s loss factor can be rewritten as ηs “

JE n´ 2 σ ψc ψl π am

(13)

where ψc and ψl are the cross section factor and length factor for the member’s loss factor, and ψc and ψl are the ratios of γc {χc and of γl {χl , respectively. The values of ψc for some special cross sections are listed in Table 1, and the values of ψl for some boundary conditions with special loads are presented in Table 2. All values of ψc and ψl are equal to 1.0 when n = 2, which proves the correctness of these expressions of ψc and ψl . Table 1. Values of ψc for some special cross sections. Cross Section Forms

Values of ψc

Rectangular Section

3 n`1

şπ

16 2 π 0

Circular Section

sinn θ cos2 θdθ bf

bf ´ b 3 bf n`1 r

Symmetrical I-section

bf ´

T-section

3 2 n´ n`1 p h q

´p ´ b

h´ 2hf n`1 q h h´ 2hf 3 p h q

s

2 rbf hn`1 `bhn`1 ´ pbf ´ bqph1 ´ hf qn`1 s 1 2 3 3 rbf h1 `bh2 ´ pbf ´ bqph1 ´ hf q3 s

Note: bf and b are the flange width and web width, respectively, of Symmetrical I-section or T-section; and hf and h are the flange height and total height, respectively, of Symmetrical I-section or T-section.

Materials 2015, 8

5304

Table 2. Values of ψl for some boundary conditions with special loads. Member’s Boundary Conditions

Load Types

Values of ψl

Simply Supported

Concentrated Load at Mid-span

3 n`1

Simply Supported Cantilever Cantilever One End Clamped and Another End with Sliding Bearing

Uniformly Distributed Load

şl

3.75ˆ4n 2 l2n`1 0

n

plx ´ x2 q dx

Concentrated Load at Cantilever End

3 n`1

Uniformly Distributed Load

5 2n`1

Concentrated Load at the End of Sliding Bearing

3 n`1

When n ‰ 2.0, it is obvious that the loss factor of the member is not only dependent on the stress amplitude but also affected by factors such as cross section forms, load types, loading positions, and boundary conditions. This indicates that the loss factor is nonlinear. Conversely, when n “ 2.0, the exponent of stress amplitude for the loss factor is equal to zero and the values of ψc and ψl are equal to 1.0; therefore, the loss factor is independent of the above factors. In this case, the loss factor is linear and Equation (12) is simplified as follows: ηs “ JE{π

(14)

2.6. Loss Tangent of Material Based on the complex damping model and only considering the material’s internal damping, the bending vibration equation for the member, as shown in Figure 1, is obtained by dynamic analysis as reported in [37] ¯ B 4 vpx, tq B 2 vpx, tq ´ 2 m ` EI ` iE I “ ppx, tq (15) c c Bt2 Bx4 where m is the member’s line density; Ic , the moment of inertia for the member’s cross section; t, the time; vpx, tq, the member’s bending vibration displacement; and ppx, tq, the distributed load along the Y-axis direction. The member’s loss factor can be described differently as 2

Ds E Ic ηs “ “ “η 2πUs EIc

(16)

By substituting Equation (12) into Equation (15), the loss tangent of the material can be expressed in the form JE n´ 2 η“ σ ψc ψl (17) π am

Materials 2015, 8

5305

3. Experimental Investigation 3.1. Materials 3.1.1. Cement The cement used in this study was ordinary Portland cement with a 28-day nominal compressive strength of 42.5 MPa. The chemical composition of cement is shown in Table 3. Table 3. Chemical composition (by mass) of cement. SiO2 (%)

Al2 O3 (%)

Fe2 O3 (%)

CaO (%)

R2 O (%)

Loss on Ignition (%)

18.73

5.88

3.37

61.89

0.54

3.03

3.1.2. Fine Aggregate The natural fine aggregate (NFA) used was river sand and it was controlled by grading to 5 mm. Its apparent density was 2514 kg/m3 , and its moisture content was 0.96%. 3.1.3. Coarse Aggregate The natural coarse aggregate (NCA) was common crushed stone, and the recycled coarse aggregate (RCA) was produced from demolished laboratory concrete samples by crushing artificially. The NCA and RCA were controlled by grading to 20 mm, and their properties are listed in Table 4. Table 4. Properties of coarse aggregates. Types

Apparent Density (kg/m3 )

Bulk Density (kg/m3 )

Moisture Content (%)

Water Absorption (%)

Crushing Index (%)

NCA

2561

1380

0.41

1.06

9.8

RCA

2509

1253

2.19

5.48

15.6

3.1.4. Modified Materials In order to improve the damping, strength, and ductility of the recycled aggregate concrete, modified materials such as polypropylene fiber (PF), steel fiber (SF), rubber powder (RP), micro-silica fume (MSF), ultrafine slag (US), and fly ash (FA, II-grade) were used. The length of PF was 19 mm and its density was 0.91 g/cm3 ; the elastic modulus and tensile strength of PF exceeded 3700 MPa and 650 MPa, respectively. The length of SF was 30 mm. The ratio of length/diameter was 43 and the PF’s tensile strength exceeded 600 MPa. The specific surface area of US was 910 m2 /kg. The RP used in this study was recycled from waste tires, and its average size was 0.84 mm and its elastic modulus was about 6 MPa. The FA was produced from a power plant and its fineness was 1.78; the SO3 content and CaO content were 0.5% and 1%, respectively. The average size of MSF was 0.21–0.26 µm, the SiO2 content of MSF was greater than 96% and its 28-day pozzolanic activity index was 90%.

Materials 2015, 8

5306

3.2. Specimen Preparation Six types of specimens were designed, and they were classified into two groups as follows: (1) The first group had three types of specimens, and it was used to study the effect of the RCA replacement ratio on the damping of concrete. Three RCA replacement ratios were considered, i.e., 0%, 30%, and 70%, and corresponding specimens were denoted as RCA-0, RCA-30, and RCA-70, respectively. (2) The second group also had three types of specimens, and it was used to study the effect of modified materials on the damping of concrete. The specimens were respectively modified by MSF + PF, RP + SF, and FA + US, and the corresponding specimens were denoted as RCA-MSF + PF, RCA-RP + SF, and RCA-FA + US, respectively. Owing to the maximum exciting force controlled by the existing electromagnetic exciter being limited, the specimens cannot be molded with the same scale as real building members. Therefore, they were designed as 80 mm (width) ˆ 80 mm (height) ˆ 1000 mm (length) beams. Table 5 presents the composition of RAC. The designed water/cement ratio was 0.5 for all proportion cases, and the additional water and water reducer were used to reach the target slump of 30 mm. The additional water was used for considering the high water absorption ratio of RCA, as shown in Table 4, and the water reducer was used to consider the high ratio of water demand of MSF, RP, and US. For each proportion case, two RC beams and six 100 mm cubic blocks were cast. These beams are prepared for the damping test and the cubic blocks are used to assess the 28-day compressive strength and split tensile strength. Table 5. Mixture proportions of recycled aggregate concretes (kg/m3 ). Types

Cement

Water

Sand

NCA

RCA

Modifiers

AW

Water Reducer

RCA-0

410

205

625

1160

0

0

0

0

RCA-30

410

205

625

812

348

0

19

0

RCA-70

410

205

625

348

812

0

44

0

RCA-MSF + PF

390

205

625

0

1160

20(MSF) + 1.2(PF)

134

7.37

RCA-RP + SF

410

205

575

0

1040

50(RP) + 120(SF)

62

3.0

RCA-FA + US

287

205

625

0

1160

82(FA) + 41(US)

50

1.0

3.3. Testing Method The test was conducted on a three-point dynamic bending testing device, as shown in Figure 2. The testing procedure was led as follows: First, a 1.0 Hz sine signal was produced by a signal-generator. Second, four different exciting force amplitudes (i.e., 50, 100, 150, and 200 N) were applied at the middle of the simply supported beam by an electromagnetic vibration exciter. Third, the force value was measured by a force transducer that was fixed under the beam, and the middle point displacement of the beam was measured by a laser transducer above the beam. Finally, all measured data were stored in a computer by a data acquisition system.

Materials 2015, 8 Materials 2015, 8

5307 5296

Figure 2. Three-point dynamic dynamic bending bending testing Figure 2. Three-point testing device. device.

Based on on the the complex complex damping damping model, model, the the loss loss tangent tangent and and elastic elastic modulus modulus of of RAC RAC can can be be calculated calculated Based by Equations Equations (17) (17) and and (18) (18) [38]. [38]. by 1 (18) η“ 1 ω2 ml ˆ tan δ v 0 1 ` p cos tan 2 δ 2 ml 0v (17) 0 ˆ 1 ˙ p0 p0 cos 2 22 2l3 E“ cos δ ` 2π f m ˆ (19) v0 Ic3 π 4 p 2l 2 2 f 2 m 4 E 0vcos (18)δ, where p0 is the exciting force amplitude; amplitude of the beam; 0 , the midpoint displacement v0 Ic the phase shift between the exciting force and the midpoint displacement; ω, the first natural radian v0 , the midpoint displacement amplitude of the beam; where p0 of is the thebeam; exciting force amplitude; frequency f , the exciting frequency.

, the phase shift between the exciting force and the midpoint displacement; , the first natural radian 3.4. Experimental Resultsf ,and the Discussion exciting frequency. frequency of the beam; 3.4.1. CompressiveResults Strength Split Tensile Strength 3.4. Experimental andand Discussion TheCompressive 28-day compressive split tensile strength are presented in Table 6. Compared with 3.4.1. Strengthstrength and Splitand Tensile Strength the compressive strength of RCA-0, those of RCA-30, RCA-70, RCA-MSF + PF, RCA-RP + SF, and The 28-day strength and split tensile strength presented Table 6. Compared with RCA-FA + US compressive were decreased by 3.2%, 6.8%, 39.7%, 50.6%,areand 27.4%, in respectively. Compared to the compressive strengthof of RCA-0, RCA-0, those those of of RCA-30, RCA-30, RCA-70, RCA-70, RCA-MSF RCA-MSF + + PF, PF, RCA-RP RCA-RP + + SF, and the split tensile strength SF, and RCA-FA ++ US USwere werealso decreased by 3.2%, 6.8%, 39.7%, 50.6%, RCA-FA decreased by 4.1%, 9.1%, 28.6%, 4.1%,and and27.4%, 29.7%,respectively. respectively.Compared to theThe splitold tensile strength thoseofof RCA-30, RCA-70, RCA-MSF + PF, RCA-RP +produced SF, and mortar adheredofonRCA-0, the surface RCA has a large number of pores and micro-cracks RCA-FA + US werelead alsotodecreased by 4.1%, 9.1%, 28.6%, 4.1%, 29.7%, respectively. by crushing, which low density and high absorption. As aand result, the crushing index and water The old mortar on the surface of RCA has a large number compared of pores and micro-cracks produced absorption of RCAadhered are increased by 59.2% and 417%, respectively, with that of NCA, shown byTable crushing, which to low density As aboth result, the crushing index and in water in 4. Thus, thelead compressive strengthand andhigh splitabsorption. tensile strength decreased with an increase the absorption of RCA are increased by 59.2% and 417%, respectively, compared with that of NCA, shown RCA replacement ratio. The modified recycled aggregate concretes with more RCAs were supplemented in Table 4. reducer, Thus, thewhich compressive strength and split tensile strength both decreased increase in with water increased the effective equivalent water/cement ratio, andwith theirancompressive the RCAdecreased replacement ratio. The modified aggregate more RCAs were strength significantly. Owing to the recycled low elastic modulus concretes of RP, the with compressive strength of supplemented reducer, the effective equivalent ratio,toand their RCA-RP + SFwith waswater lowest, but thewhich split increased tensile strength of RCA-RP + SFwater/cement was almost equal that of compressive strength decreased significantly. Owing to the low elastic modulus of RP, the compressive RCA-0 due to the reinforcement of SF. strength of RCA-RP + SF was lowest, but the split tensile strength of RCA-RP + SF was almost equal to that of RCA-0 due to the reinforcement of SF.

Materials 2015, 8

5308 Table 6. The 28-day compressive strength and split tensile strength.

Specimens Compressive Strength/Standard deviation (MPa) Split Tensile Strength/Standard deviation (MPa)

RCA-0

RCA-30

RCA-70

RCA-MSF + PF

RCA-RP + SF

RCA-FA + US

50.4/1.6

48.8/1.8

47.0/0.4

30.4/1.5

24.9/1.1

36.6/1.4

5.36/0.45 5.14/0.14

4.87/0.38

3.83/0.34

5.15/0.40

3.77/0.27

3.4.2. Loss Tangent and Elastic Modulus The loss tangent and elastic modulus of RAC are shown in Table 7. It is found that the loss tangent for all types of RAC increases with the exciting force amplitude even if the beams are under low-amplitude vibrations. Compared with the loss tangents at the exciting force amplitude of 50 N, the loss tangents at the exciting force amplitude of 200 N increased by 5.8% (RCA-0), 3.9% (RCA-30), 6.0% (RCA-70), 20.1% (RCA-MSF + PF), 16.0% (RCA-RP + SF), and 13.6% (RCA-FA + US), respectively. The loss tangent increases slightly with the RCA replacement ratio and increases significantly when the RAC was added with modified admixtures. Compared with the loss tangent of RCA-0 at the exciting force amplitude of 200 N, the loss tangents increased by 1.2% (RCA-30), 5.5% (RCA-70), 20.1% (RCA-MSF + PF), 71.0% (RCA-RP + SF), and 47.4% (RCA-FA + US), respectively. The elastic modulus at the exciting force amplitude of 200 N is reduced by 5.1% (RCA-70), 16.7% (RCA-MSF + PF), 16.2% (RCA-RP + SF), and 13.6% (RCA-FA + US), compared with that of RCA-0. In general, the elastic modulus decreased slightly with the RCA replacement ratio, and decreased markedly when the RAC was added with modified admixtures. However, no obvious regularity is found about the relationship between the elastic modulus and the exciting force amplitude at low-amplitude vibrations. Table 7. The loss tangent and elastic modulus of recycled aggregate concrete. Specimens

Elastic Modulus (104 N/mm2 )

Loss Tangent (%) 50 N

100 N

150 N

200 N

50 N

100 N

150 N

200 N

RCA-0

5.50

5.63

5.66

5.82

3.68

3.55

3.36

3.54

RCA-30

5.67

5.71

5.83

5.89

3.63

3.55

3.49

3.54

RCA-70

5.79

5.93

6.00

6.14

3.00

3.30

3.27

3.36

RAC-MSF + PF

5.82

6.10

6.62

6.99

2.92

3.03

3.02

2.95

RAC-RP + SF

8.58

9.31

9.72

9.95

2.77

2.87

2.75

2.97

RAC-FA + US

7.55

7.88

8.28

8.58

3.59

3.08

3.29

3.06

3.4.3. Energy Coefficient and Exponent When a concentrated force with amplitude p0 is applied at the mid-span of a simply supported beam with a rectangular cross section, the maximum elastic stress of the beam is σam “

3p0 l 2br hr 2

(20)

Materials 2015, 8

5309

where br and hr are the width and height of the rectangular cross section, respectively. By substituting Equation (19) and the values of ψc and ψl into Equation (16), the loss tangent takes the form ˙n´ 2 ˆ 9JE 3p0 l (21) η“ πpn ` 1q2 2br hr 2 The numerical fitting for the relationship between the loss tangent and the exciting force amplitude was performed according to Equation (20) by Matlab programming, and the damping energy coefficient and exponent of RAC are obtained, as shown in Table 8. Table 8. Damping energy coefficient and exponent of recycled aggregate concrete. Specimens

Damping Energy Coefficient J (ˆ10´6 MPa´1 )

Damping Energy Exponent n

Correlation Coefficient R2

RCA-0

5.39

2.04

0.862

RCA-30

5.41

2.03

0.898

RCA-70

6.29

2.04

0.957

RCA-MSF + PF

9.53

2.10

0.969

RCA-RP + SF

13.04

2.14

0.996

RCA-FA + US

8.73

2.14

0.937

The influence of the RCA replacement ratio on the damping energy exponent is slight, and the value of n is about 2.04. The influence of modified admixtures on the damping energy exponent is obvious, and the value of n is increased to 2.10–2.14. It should be noted that all values of n are not equal to 2.0, indicating that the recycled aggregate concrete is not a type of completely elastic material, as we usually think, even at low bending stress amplitudes. Compared with the damping energy coefficient of NAC, those of RACs are increased by 0.4% (RCA-30), 16.7% (RCA-70), 76.8% (RCA-MSF + PF), 141.9% (RCA-RP + SF), and 62% (RCA-FA + US), respectively. The damping energy coefficient of the RAC is greater than that of the NAC, implying that the energy dissipation capacity of the RAC is greater than that of the NAC under the same conditions. 4. Conclusions The relationship between the loss factor and the stress amplitude of a member is derived when the member is at a low-amplitude bending vibration. The loss factor of the member depends not only on the stress amplitude, but also factors such as the cross section shapes, boundary conditions, load types, and loading positions. The loss tangent of RAC is obtained through experimental investigations. The loss tangent increases slightly with the bending stress amplitude and with the RCA replacement ratio, and increases significantly with adding modified admixtures. The damping energy coefficient and exponent are obtained by numerical fitting to determine an explicit stress amplitude-dependent damping function of RAC. The damping energy exponent of RAC is not equal to 2.0, indicating that the damping of RAC, especially the RAC with modified admixtures, is

Materials 2015, 8

5310

nonlinear. In addition, compared with NAC, the damping energy coefficient of RAC is increased, and it is further increased by modified admixtures. Acknowledgments This work is supported by National Nature Science Foundation of China (Grant NO. 51422804, 51308340, 51308322), Program for New Century Excellent Talents in University (NCET-13-0171), and Zhejiang Provincial Natural Science Foundation of China (Grant NO. Y1110184) Author Contributions T.L. and J.X. conceived and designed the experiment; D.Z. and C.L. conducted the experiment and analyzed the data; C.L. and Q.Y. derived the stress amplitude-dependent damping function; C.L. and D.Z. wrote the paper. Conflicts of Interest The authors declare no conflict of interest. Notation ψc ψl n J E σam

the cross section factor for the member’s loss factor the length factor for the member’s loss factor damping energy exponent damping energy coefficient, MPa´1 elastic modulus of material, MPa the maximum stress of the member, MPa

Appendix Stress Amplitude-Dependent Damping Function ηs “

JE n´ 2 σ ψc ψl π am

(A1)

References 1. Fu, X.L.; Chung, D.D.L. Vibration damping admixtures for cement. Cem. Concr. Res. 1996, 26, 69–75. [CrossRef] 2. Wang, Y.; Chung, D.D.L. Effects of sand and silica fume on the vibration damping behavior of cement. Cem. Concr. Res. 1998, 28, 1353–1356. [CrossRef] 3. Chung, D.D.L. Flexible graphite for gasketing, adsorption, electromagnetic interference shielding, vibration damping, electrochemical applications, and stress sensing. J. Mater. Eng. Perform. 2000, 9, 161–163. [CrossRef] 4. Chung, D.D.L. Structural composite materials tailored for damping. J. Alloy. Compd. 2003, 355, 216–223. [CrossRef]

Materials 2015, 8

5311

5. Neithalath, N.; Weiss, J.; Olek, J. Acoustic performance and damping behavior of cellulose-cement composites. Cem. Concr. Compos. 2004, 26, 359–370. [CrossRef] 6. Ou, J.P.; Liu, T.J.; Li, J.L. Analysis of the damping behavior and microstructure of cement matrix with silane-treated silica fume. J. Wuhan Univ. Technol. Mater. 2006, 21, 1–5. 7. Ou, J.P.; Liu, T.J.; Li, J.L. Dynamic and seismic property experiments of high damping concrete and its frame models. J. Wuhan Univ. Technol. Mater. 2008, 23, 1–6. [CrossRef] 8. Swamy, N.; Rigby, G. Dynamic properties of hardened paste, mortar and concrete. Mater. Constr. 1971, 4, 13–40. [CrossRef] 9. Jordan, R.W. The effect of stress, frequency, curing, mix and age upon the damping of concrete. Mag. Concr. Res. 1980, 32, 195–205. [CrossRef] 10. Ke, G.J.; Dai, M.; Peng, H.; Chen, Z.F. Damping ratio of concrete after its coarse aggregate surface is treated by viscoelastic materials. J. Build. Mater. 2009, 12, 605–608. 11. Lazan, B.J. Damping of Material and Members in Structural Mechanics; Pergamon Press: London, UK, 1968. 12. Kume, Y.; Hashimoto, F.; Maeda, S. Material damping of cantilever beams. J. Sound Vib. 1982, 80, 1–10. [CrossRef] 13. Gounaris, G.D.; Anifantis, N.K. Structural damping determination by finite element approach. Comput. Struct. 1999, 73, 445–452. [CrossRef] 14. Gounaris, G.D.; Antonakakis, E.; Papadopoulos, C.A. Hysteretic damping of structures vibrating at resonance: An iterative complex eigensolution method based on damping-stress relation. Comput. Struct. 2007, 85, 1858–1868. [CrossRef] 15. Hwang, T.H.; Scribner, C.F. R/C member cyclic response during various loadings. J. Struct. Eng. 1984, 110, 477–489. [CrossRef] 16. Darwin, D.; Nmai, C.K. Energy dissipation in RC beams under cyclic load. J. Struct. Eng. 1986, 112, 1829–1846. [CrossRef] 17. Wen, J.; Wang, Y.F. Calculation of material damping of reinforced concrete cantilever beams. China Civ. Eng. J. 2008, 110, 477–489. 18. Fang, J.Q.; Jeary, A.P.; Li, Q.S.; Wong, C.K. Random damping in buildings and its AR model. J. Wind Eng. Ind. Aerodyn. 1999, 79, 159–167. [CrossRef] 19. Jeary, A.P. Damping in structures. J. Wind Eng. Ind. Aerodyn. 1997, 72, 345–355. [CrossRef] 20. Li, Q.S.; Yang, K.; Wong, C.K. The effect of amplitude-dependent damping on wind-induced vibrations of a super tall building. J. Wind Eng. Ind. Aerodyn. 2003, 91, 1175–1198. [CrossRef] 21. Li, Q.S.; Liu, D.K.; Fang, J.Q.; Jeary, A.P.; Wong, C.K. Damping in building: Its neural network model and AR model. Eng. Struct. 2000, 22, 1216–1223. [CrossRef] 22. Lee, G.C.; Choi, H.B. Study on interfacial transition zone properties of recycled aggregate by micro-hardness test. Constr. Build. Mater. 2013, 40, 455–460. [CrossRef] 23. Nagataki, S.; Gokce, A.; Saeki, T.; Hisada, M. Assessment of recycling process induced damage sensitivity of recycled concrete aggregates. Cem. Concr. Res. 2004, 34, 965–971. [CrossRef] 24. Choi, H.B.; Kim, B.J.; Kang, K.I. Absorption properties and shape of micro-cracks incurred in recycled aggregate. Archit. Inst. Korea 2011, 27, 83–90.

Materials 2015, 8

5312

25. Xiao, J.Z.; Li, J.B.; Zhang, C. Mechanical properties of recycled aggregate concrete under uniaxial loading. Cem. Concr. Res. 2005, 35, 1187–1194. [CrossRef] 26. Lima, C.; Caggiano, A.; Faella, C.; Martinelli, E.; Pepe, M.; Realfonzo, R. Physical properties and mechanical behaviour of concrete made with recycled aggregates and fly ash. Constr. Build. Mater. 2013, 47, 547–559. [CrossRef] 27. Koenders, E.A.B.; Pepe, M.; Martinelli, E. Compressive strength and hydration processes of concrete with recycled aggregates. Cem. Concr. Res. 2014, 56, 203–212. [CrossRef] 28. Levy, S.M.; Helene, P. Durability of recycled aggregates concrete: A safe way to sustainable development. Cem. Concr. Res. 2004, 34, 1975–1980. [CrossRef] 29. Bravo, M.; de Brito, J.; Pontes, J.; Evangelista, L. Durability performance of concrete with recycled aggregates from construction and demolition waste plants. Constr. Build. Mater. 2015, 77, 357–369. [CrossRef] 30. Fathifazl, G.; Razaqpur, A.G.; Isgor, O.B.; Abbas, A.; Fournier, B.; Foo, S. Creep and drying shrinkage characteristics of concrete produced with coarse recycled concrete aggregate. Cem. Concr. Compos. 2011, 33, 1026–1037. [CrossRef] 31. Yang, K.H.; Chung, H.S.; Ashour, A. Influence of type and replacement level of recycled aggregates on concrete properties. ACI Mater. J. 2008, 105, 289–296. 32. Xiao, J.Z.; Li, H.; Yang, Z.J. Fatigue behavior of recycled aggregate concrete under compression and bending cyclic loadings. Constr. Build. Mater. 2013, 38, 681–688. [CrossRef] 33. Xiao, J.Z.; Li, L.; Shen, L.M.; Poon, C.S. Compressive behaviour of recycled aggregate concrete under impact loading. Cem. Concr. Res. 2015, 71, 46–55. [CrossRef] 34. Sidorova, A.; Vazquez-Ramonich, E.; Barra-Bizinotto, M.; Roa-Rovira, J.J.; Jimenez-Pique, E. Study of the recycled aggregates nature’s influence on the aggregate–cement paste interface and ITZ. Constr. Build. Mater. 2014, 68, 677–684. [CrossRef] 35. Brand, A.S.; Roesler, J.R.; Salas, A. Initial moisture and mixing effects on higher quality recycled coarse aggregate concrete. Constr. Build. Mater. 2015, 79, 83–89. [CrossRef] 36. Myklestad, N.O. The concept of complex damping. J. Appl. Mech. 1952, 19, 20–30. 37. Clough, R.W.; Penzien, J. Dynamics of Structures, 3rd ed.; Computers and Structures, Inc.: New York, NY, USA, 2003. 38. Liu, T.J. Self-Reinforced Damping Concrete and High Damping Structures. Ph.D. Thesis, Harbin Institute of Technology, Harbin, China, 2004. © 2015 by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution license (http://creativecommons.org/licenses/by/4.0/).